Loading in 2 Seconds...
Loading in 2 Seconds...
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author. While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
Concrete Technology Surface Finishes on Concrete Defects in Concrete Lecture 21 Eng: Eyad Haddad
Surface Finishes on Concrete • Concrete can be given many different surface finishes including: • BROOMING • COLOURING • PATTERNING or • POLISHING • CONCRETE In order to minimize problems arising when using any form of colored concrete for domestic paving, either a minimum grade of 25 MPa or concrete containing not less than 280 kg of cement/m3 should be used. Other forms of decorative concrete, or in commercial work, will normally require a higher grade of concrete.
Surface Finishes on Concrete • Concrete can be given many different surface finishes including: • BROOMING • COLOURING • PATTERNING or • POLISHING • CONCRETE In order to minimize problems arising when using any form of colored concrete for domestic paving, either a minimum grade of 25 MPa or concrete containing not less than 280 kg of cement/m3 should be used. Other forms of decorative concrete, or in commercial work, will normally require a higher grade of concrete. TEST PANELS To find out how a color or pattern will look always do a small test area before beginning the bulk of the work. CURING COLOURED CONCRETE Curing is the most important step in coloring concrete. The concrete surface must stay evenly moist or the color will be uneven. Poorly cured concrete can even affect a painted concrete surface.
Surface Finishes on Concrete • COLOURED FINISHES: • There are four ways to colour concrete: • 1. The Dry-Shake Method: • The dry-shake method uses a mixture of a mineral oxide pigment (or color), cement and specially graded fine aggregates. • The color is added when compaction, screeding and bleeding has finished, as part of finishing. • Uniform reliable results are best achieved if the concrete is supplied pre-mixed by the supplier using weight batched dry components. • Shake 2/3 of the dry material onto the concrete surface, spreading it evenly with a float. Leave for a minute or so to soak up some moisture. • Shake the last 1/3 of the dry material onto the concrete at right angles to the first application and again after it has dampened up, spread evenly with a float. • The two applications help to give a more uniform color and thickness. • Re-tool any edges and joints. After a while the surface must be re-floated.
Surface Finishes on Concrete • 2. Full depth colour: • The color is added to the concrete during mixing so all the concrete is colored, then the concrete is compacted and finished as for normal concrete. • The color pigment additives should generally be in the range of 3–7% by weight of the cement. • Higher quantities may affect the strength and durability of the concrete. • Check manufacturer details for color selection. • Each batch must be accurately proportioned, thoroughly mixed and well floated to give an even color. • The color of the cement powder may effect the shade of the final color, (ie a dark grey cement may affect light colors).
Surface Finishes on Concrete • 3. Applied finishes: • Applied finishes, including paints, tinted sealers and trowelled-on coatings provide a wide range of colors and are easily applied to hardened dry concrete. • Paint finishes are either water-based or solvent based. They will wear easily and will need to be reapplied periodically. • 4. Chemical stains: • A chemical stain soaks into the concrete surface and colors its, only wearing away as much as the surface does. • There is only a limited color range in concrete stains.
Surface Finishes on Concrete 5. Stamped pattern finish: A number of DIFFERENT PATTERNS can be stamped into the surface of setting concrete. (cobblestone, slate, tile, brick tile and timber finishes) The concrete is placed and compacted normally, and floated once. The surface must then be broomed to give a non-slip finish. Use small handstamps for the edges and any difficult to reach areas. Brick, or tile finishes, (stencilled concrete) can be obtained by floating a paper template into the concrete surface before applying a dry shake. The template forms the mortar lines.
Surface Finishes on Concrete • 6. Exposed aggregate finish: • An exposed aggregate finish can be an attractive decorative finish. Different sizes and colors of aggregates allow many different looks. • The concrete can be made as normal, and the course aggregate exposed. This is done by waiting until the surface is firm, but not dry, then brush, wash or broom away any cement paste until the aggregates are exposed. Then cure the concrete. • A surface retardant can be used to aid the process.
Surface Finishes on Concrete • Methods of exposed aggregate finish: (2 Methods) • Method A • Place, compact and level the concrete to about 10 mm below the top of the forms. • Spread selected aggregates over the concrete in a layer and press them into the • concrete until completely covered. • Method B • Place, compact and level concrete to about 5 mm below the top of the forms. • Mix a 'Topping Coat' – A mix of aggregates and cement paste in the ratio 2:1. • Use only enough water to make the coat workable. • Spread the topping over the concrete, level, tamp down and finish with a trowel.
Surface Finishes on Concrete • FOR BOTH METHODS • leave the concrete until the cement paste on the surface is firm, but not dry, then brush or with a fine mist spray wash away some of the cement paste covering the aggregates. • In both cases extra cleaning can be done with a dilute solution of hydrochloric acid. • The solution should be 1 part acid to 20 parts water. Wet the concrete first and rinse off thoroughly afterwards. Observe safety procedures. • Different colors of cement can be used to get a better effect. For instance a white or off- white cement may be used with a light stone where a grey cement may create a clash of colors. A BROOMED FINISH To give a skid-resistance surface a stiff, or soft, bristle broom can simply be drawn across the surface of concrete. The broom can be drawn in straight or 's' shape lines.
Surface Finishes on Concrete • POLISHED CONCRETE • Polished concrete is a finish used on the interior and exterior of dwellings. A variety of finishes can be achieved by using different techniques or products. • The different finishes can be achieved by using liquid polishes, latex coatings, chemical sealers, grinding to expose the aggregates, colors, stains and special aggregates to achieve other desired effects. THE END
Defects in Concrete • Some defects are obvious only to a trained eye, others, such as cracking, are obvious to anyone. • 1. COLOUR VARIATION: • Difference in color across the surface of concrete. May appear as patches of light and dark. • Causes: Uneven or variable curing conditions. • Prevention: Use an even concrete mix when placing, compacting and finishing and keep • concrete evenly moist. Do not use driers. • Repair: To hide the variation a SURFACE COATING can be applied. • Rectification of color variation from stains is a very difficult operation and may need repeated • gentle treatments with a weak acid.
Defects in Concrete • 2. CRAZING: • A network of fine cracks across the surface of concrete. • Causes: Crazing is caused by minor surface shrinkage in rapid drying conditions. (ie Low • humidity and hot temperatures, or alternate wetting and drying.) • Prevention: Finish and cure concrete correctly. • Repair: Repair may not be necessary because crazing will not weaken concrete. If the crazing • looks too bad then a surface coating of a paint or other overlay sealer can be applied to cover • and/or minimize the effect of the cracks.
Defects in Concrete • 3. DUSTING: • A fine powder on the concrete surface which comes off on your fingers. • Causes: Finishing before the bleed water has dried. Also finishing during the rain. Not • curing properly, or the surface is drying too quickly. • Concrete subject to severe abrasion or of too low a grade for the end use. • Prevention: • Let any bleed water dry up before trowelling or in cold conditions remove the water. • Cure correctly. • Protect concrete from drying out too quickly in hot or windy conditions. • For harsh conditions use a stronger concrete. Repair: dusting concrete surfaces result from inadequate attention to prescribed placement and finishing practices, the addition of excess water, working in of bleedwater, the inadequate compaction and curing of concrete. If the surface is showing significant wear distress it is essential to remove all loose material by grinding or scrapping the surface to a sound base and then applying a suitable topping.
Defects in Concrete • 4. RAIN DAMAGE • The surface has bits washed away or many small dents. • Causes: Heavy rain while concrete is setting or rainwater being allowed to run across the • concrete surface. • Prevention: • Cover the concrete if it is raining or it looks like it might rain. • Don’t lay concrete if it looks like it might rain. • Repair If the concrete has not hardened and damage is minimal the surface can be refloated and re-trowelled taking care not to overwork excess water into the surface. NOTE: If the concrete has hardened it may be possible to grind or scrape the minimal amount of the surface layer and apply a topping layer of new concrete or a repair compound. This may not always be possible and should only be done with expert advice.
Defects in Concrete • 5. SPALLING: • When the slab edges and joints chip or break leaving an elongated cavity. • Causes: • Edges of joints break because of heavy loads or impact with hard objects. • Entry of hard objects, such as stones, into joints may cause spalling when the concrete expands. • Poor compaction of concrete at joints. • Prevention: • Design the joints carefully. • Keep joints free from rubbish. Keep heavy loads away from the joints and edges until they • have properly hardened. Ensure proper compaction. • Repair: For small spalled areas: scrape, chip or grind away the weak areas until you reach • sound concrete, making sure you brush the old concrete clean of any loose material. Then refill • the area with new concrete or repair mortar. Compact, finish and cure the new patch carefully. • Care should be taken that all joints be maintained and not filled. • For large spalled areas: seek expert advice
Defects in Concrete • 6. EFFLORESCENCE: • A white crystalline deposit sometimes found on the surface of concrete soon after it is • finished. • Causes: • Sometimes mineral salts are dissolved in water. • Excess bleeding can also result in efflorescence. • Prevention: • Use clean, salt-free water and washed sands. • Avoid excessive bleeding. • Repair: • Remove efflorescence by dry brushing and washing with clean water. • Do not use a wire brush. • Wash with a dilute solution of hydrochloric acid.
Defects in Concrete • 7. HONEYCOMBING: • When too much coarse aggregate appears on the surface. • Causes: • Poor compaction, segregation during placing or paste leakage from forms. A poor concrete mix with not enough fine aggregate causing a rocky mix. • Prevention: • Use a better mix design. • Take care during placing concrete to avoid segregation. • Compact concrete properly. • Good watertight formwork. • Repair: If honeycombing happens only on the surface it can be rendered. If honeycombing happens throughout the concrete it may need to be removed and replaced. The surface may require rendering. • (Rendering means to cover the surface with a layer of mortar).
Defects in Concrete 8. BLISTERING: Blisters are hollow, low profile bumps on the concrete Surface filled with either air or bleed water. Causes: They are caused when the fresh concrete surface is sealed by trowelling while trapping air or bleed water under the surface. This may particularly occur in thick slabs or on hot, windy days when the surface is prone to drying out. Prevention: After placing, screeding and floating leave the concrete as long as possible before trowelling, which seals the surface. Cure to prevent evaporation. If blisters are forming delay trowelling as long as possible and take steps to reduce evaporation. Repair: Grind off the weakened layer to an even finish.